£â€œ Springer-Verlag 1997 The Elastic-Plastic Finite Element ... T-integral...
Embed Size (px)
Transcript of £â€œ Springer-Verlag 1997 The Elastic-Plastic Finite Element ... T-integral...
The Elastic-Plastic Finite Element Alternating Method (EPFEAM) and the prediction of fracture under WFD conditions in aircraft structures Part III: Computational predictions of the NIST multiple site damage experimental results
L. Wang, F. W. Brust, S. N. Atluri
Abstract This report provides a summary of the Elastic- Plastic Finite Element Alternating Method (EPFEAM), the T�-integral fracture mechanics parameter, and the use of both the tools to predict the residual strength of aircraft panels with multiple-site damage. Because this report is meant to be self-contained and each of the three subjects is a considerable research topic in itself, the report is written in three parts. Part I, EPFEAM Theory provides a summary of the elastic-plastic ®nite element alternating method (EPFEAM) and the algorithms for fracture analysis and crack growth predictions. Part II, Fracture and the T�- Integral Parameter provides a complete description of the T�-integral fracture parameter including a detailed dis- cussion of the theoretical basis of T� and the practical aspects of its use for fracture predictions. Finally, Part III, Computational Predictions of the NIST Multiple Site Damage Experimental Results provides a series of pre- dictions of a number of fracture tests performed at the National Institute of Standards and Technology (NIST). These predictions are then compared with the experi- mental data, thus validating the present model for com- puting the residual strength under wide-spread-fatigue damage conditions.
The reader that is interested in all the topics can study all the three self-contained parts, while the reader that is only interested in the practical aspects of fracture pre- dictions using these methods can read only Part III.
This is the Part III report, ``Computational Predictions of the NIST Multiple Site Damage Experimental Results''.
1 Introduction The economic environment in the United States (and the global economy for that matter), that has persisted for more than ten years, is focused on controlling and con- taining costs. This attitude, which has been prevalent in industry for years and now is the focus of the US gov- ernment as well, has led to a concept called life extension. Life extension refers to the concept of continuing to use structures long beyond the original intended design life. As long as the maintenance costs associated with extend- ing the life of an aging component or process remain lower than the huge capital expenditures associated with de- signing and building a new structure, the life extension philosophy will continue. Examples of industries which are actively extending the life of processes include the fossil and nuclear power industries which are attempting to use plants far beyond their intended design life. Also, the aerospace industry, both commercial and military, is at- tempting to use aircraft far beyond their initial design lives. Indeed, methods to evaluate the structural integrity so that life extension of the aging commercial airline ¯eet may continue is the focus of this report.
In order to de®ne the maintenance requirements of an aging aircraft to ensure its' continued structural integrity and safety, advanced analytical tools for life and residual strength prediction are necessary. The FAA has been charged with the development of a wide range of tools for assuring the integrity of aging aircraft. These tools include, among many others, advanced and accurate non-destruc- tive inspection methods, and fracture analysis techniques. The latter is the subject of this report. The FAA Center of Excellence at Georgia Tech has been involved with the development of advanced computational methods to per- mit the evaluation of structural integrity of aging aircraft in a rapid, accurate, and ef®cient way. Three major topics of development are discussed in this report: EPFEAM, Fracture, and Predictive methods.
This report is written in three parts. Part I, EPFEAM Theory provides a summary of the elastic-plastic ®nite element alternating method (EPFEAM) and the algorithms for fracture analysis and crack growth predictions. Part II, Fracture and the T�-Integral Parameter provides a com- plete description of the T�-integral fracture parameter including a detailed discussion of the theoretical basis of T� and the practical aspects of its use for fracture pre- dictions. Finally, Part III, Computational Predictions of the NIST Multiple Site Damage Experimental Results provides a series of predictions of a number of fracture tests per-
Originals Computational Mechanics 20 (1997) 199 ± 212 Ó Springer-Verlag 1997
Communicated by G. Yagwa, 31 October 1996
L. Wang, F. W. Brust, S. N. Atluri FAA Center of Excellence for Computational Modeling of Aircraft Structures, Computational Modeling Center, Georgia Institute of Technology, A. French Building, Atlanta, Georgia 30332-0356, USA
Correspondence to: S. N. Atluri
The authors would like to acknowledge the recommendations and participation of Mr. Chris Seher and Drs. Paul Tan and Cathy Bigelow of the FAA Technical Center. The useful discussions with Mr. T. Swift and Dr. J. Lincoln over the course of this work are thankfully acknowledged. Dr. Roland deWit of NIST graciously provided computer disks of the tests that he directed at NIST, in addition to providing insight into the results.
formed at the National Institute of Standards and Tech- nology (NIST). These predictions are then compared with the experimental data, thus validating the computational model.
This report focuses on the Part III topic in this report series, ``Computational Predictions of the NIST Multiple Site Damage Experimental Results''.
2 Overview of Part III ``Application predictions of the NIST multiple site damage experiments'' This Part III report of this series provides validation of the EPFEAM method (Part I) and the use of the T�-integral (Part II). The validation is made by comparing predictions of residual strength using these techniques, to experi- mental data produced by The National Institute of Stan- dards and Technology (NIST). The experimental data was developed on large panels which contained a large main crack with Multiple Site Damage (MSD) cracks ahead of the main crack. The predictions provided here are true predictions, i.e. no `fudging' of either the experimental data or the analysis predictions are made to make the predictions look better. Before providing the validation predictions it is useful to present a short overview of practical elastic-plastic fracture mechanics and the current state-of-the-art. The reader is referred to the Part I for details regarding the EPFEAM method development and improvements made here, and to the Part II for details regarding the T�-integral development.
The practical development of elastic-plastic fracture mechanics in the United States was driven primarily by the needs of the Nuclear industry which uses very ductile stainless steels for its piping systems. The nuclear regu- latory authorities permit utilities that are attempting to have a plant certi®ed, to reduce or eliminate expensive pipe whip restraints if the pipe `Leak Before Break' criteria can be met. This requires elastic-plastic fracture mechan- ics methods which are based on J-integral Tearing theory1. A complete summary of the philosophy behind the phe- nomenological J-Tearing method has been summarized by Hutchinson (1983). Hutchinson (1983) also points out explicitly the limitations of J-Tearing Theory. These limi- tations include; (i) only monotonic loading can be con- sidered and (ii) only small amounts of crack growth can be permitted. Despite these limitations a very large data base exists (see Wilkowski et al. 1995) which clearly shows that conservative predictions can be expected if a lower bound (compact specimen) J-Resistance curve is used to predict monotonic loading of one single crack to fracture in a pipe. A large ongoing program (Hopper et al. 1992) shows that J-theory cannot account for cyclic effects. Most impor-
tantly for aerospace applications, a far ®eld J value has no meaning for a large crack with MSD ahead of it.
Practical methods for predicting the residual strength of the MSD problem include the plastic zone technique (Swift 1985), the crack tip opening angle (CTOA) method (Newman et al. 1993), and the T�-integral method (Pyo et al. 1994a, 1994b; Singh et al. 1994; Brust 1995a). The plastic zone method predicts that the main crack will link with an MSD crack if their plastic zones overlap. The plastic zones are estimated using an elastic analogy such as an Irwin estimate. However, the Irwin estimate of the plastic zone size is not very accurate, especially for hard- ening materials. Moreover, there is no theoretical justi®- cation for choosing plastic zone overlaps as a link-up criterion. The CTOA method, which requires a rather de- tailed ®nite element analysis to apply, has been shown to be able to predict MSD failures. However, the CTOA is ®nite element mesh size dependent in general and often requires expensive analyses due to the need for extreme mesh re®nement. Moreover, CTOA is a geometric pa- rameter and cannot be used under more general fracture conditions such as cyclic loading and rate dependent fracture. Furthermore, the CTOA for fracture initiation and stable growth is measured in small planar specimens, wherein the crack axis lies in the plane of the specimen and the crack plane is perpendicular to the plane of the specimen. In this case, the CTOA has a reasonably clear physical basis. However, for cracks in cylindrical-shell type fuselage structures, and when such cracks bulge, the CTOA and the plane in which it should be measured are ambiguous. Thus, the implementation of a critical CTOA for fra